See discussions, stats, and author profiles for this publication at: https://www.researchgate.net/publication/302921261
Cu0.8Mg2.1Si2O6 : A copper-bearing silicate with the low-clinopyroxene structure Article in Mineralogical Magazine · April 2016 DOI: 10.1180/minmag.2016.080.002
4 authors, including: Lei Ding
Claire V. Colin
Oak Ridge National Laboratory
Université Grenoble Alpes
43 PUBLICATIONS 373 CITATIONS
109 PUBLICATIONS 958 CITATIONS
Pierre Bordet French National Centre for Scientific Research 339 PUBLICATIONS 5,950 CITATIONS SEE PROFILE
Some of the authors of this publication are also working on these related projects:
Low Dimensional Magnetic Study View project
Triangular Lattice Antiferromagnets View project
All content following this page was uploaded by Lei Ding on 06 March 2018. The user has requested enhancement of the downloaded file.
Mineralogical Magazine, April 2016, Vol. 80(2), pp. 325–335
Cu0.8Mg1.2Si2O6 : a copper-bearing silicate with the low-clinopyroxene structure LEI DING, CÉLINE DARIE, CLAIRE V. COLIN AND PIERRE BORDET,* Université Grenoble Alpes, Institut Néel, Grenoble, 38042, France CNRS, Institut Néel, Grenoble, 38042, France [Received 18 January 2015; Accepted 20 May 2015; Associate Editor: David Hibbs] ABSTR ACT
The Cu0.8Mg1.2Si2O6 pyroxene has been synthesized using a soft chemistry method. Its crystal structure was determined from powder X-ray diffraction data. Cu0.8Mg1.2Si2O6 crystallizes with the lowclinopyroxene monoclinic structure (space group P21/c). The role of the Jahn-Teller-distorted Cu2+ cation on the stability of this strongly distorted structure is investigated. Cu2+ shows a strong preference for the M2 site, attributed to a better adaptation of its JT-distorted coordination polyhedron to this already distorted and more flexible site. Comparison with previously reported compounds indicates that increasing the Cu content enhances the M2 site distortion, eventually leading to symmetry lowering from orthorhombic Pbca to monoclinic P21/c. These observations bring new insight into the mechanisms of formation and chemical composition of pyroxene minerals in the presence of JT cations. K E Y WO R D S : pyroxene, crystal structure, Jahn-Teller effect.
Introduction COMPOUNDS of the pyroxene family form one of the most abundant mineral species in the Earth’s crust and upper mantle, and have therefore been subject to a wealth of detailed studies investigating their structures and crystallo-chemistry, depending on composition, formation conditions, and so on. Pyroxene compounds with the chemical formulas M2M1Si2O6 (M1 = di- or trivalent transition metals, M2 = mono- or divalent metals) are generally found in three main forms, orthopyroxene, high clinopyroxene and low clinopyroxene, with space groups Pbca, C2/c and P21/c, respectively. Their structures are built up by chains of edgesharing M1 and M2 octahedra aligned along the c axis, linked by chains of SiO4 tetrahedra, and considerable effort has been given to understand the relation between the pyroxene composition and its structural topology (Cameron and Papike, 1981; Redhammer and Roth, 2004; Thompson and Downs, 2003, 2004; Thompson et al., 2005). In
*E-mail: [email protected]
© 2016 The Mineralogical Society
this regard, pyroxenes containing Jahn-Teller (JT) cations have been subject to particular attention. Difficulty in accommodating the corresponding polyhedral distortions may play a role in the ability of pyroxenes to contain large amounts of JT cations. Recently, pyroxenes containing magnetic cations have attracted new interest from a different viewpoint because some of them were found to present multiferroic properties (Jodlauk et al., 2007; Kim et al., 2012; Redhammer et al., 2011, 2013), magnetoelectric effects (Nenert et al., 2010a,b; Redhammer et al., 2009), and quasione-dimensional (Q1D) magnetic behaviour (Valenti et al., 2002). These physical properties are due to their unique crystal structure. Competition between inter- and intra-chain magnetic interactions leads to magnetic frustration and the appearance of various exotic magnetic properties such as a spin singlet ground state (Sasago et al., 1995) and spin-Peierls transitions (Isobe et al., 2002). In this respect, copper-containing pyroxenes are of foremost interest due to the spin ½ of Cu2+ cations, which could lead to enhanced quantum effects. According to previous investigations, the magnetic configuration in pyroxene compounds can be
LEI DING ET AL.
changed via chemical substitution at the M1 and/or M2 sites. In the case of CaCuGe2O6 the behaviour of magnetization was interpreted as due to a spinsinglet ground state (Sasago et al., 1995). Ab initio calculations indicated that this behaviour derives from intra-chain interactions of Cu2+ dimers (Valenti et al., 2002). Later on, Redhammer et al. (2005) showed that CaCuGe2O6 has the clinopyroxene structure, space group P21/c, at room temperature. As magnetic properties are influenced strongly by interatomic distances in this family of materials, it is tempting to look for compounds where Ge cations are substituted by smaller Si cations. To our knowledge, CaCuSi2O6 preparation was never reported and, despite many attempts, we were unable to synthesize it. For the larger Ba cation, BaCuSi2O6 adopts the Han purple crystal structure (Finger et al., 1989; Sparta and Roth, 2004). Attempts to synthesize MgCuSi2O6 by soft chemistry methods lead to the preparation of a compound with a composition close to CuMgSi2O6. The existence of the CuMgSi2O6 pyroxene was reported by Breuer et al. (1986), but only the cell parameters and a tentative space group were given. In fact, the only other Cu-bearing pyroxene silicate for which a complete structure analysis was reported is the orthopyroxene (Cu0.44Mg1.56)Si2O6 (Tachi et al., 1997), space group Pbca. It is important to note that, at variance with CaCuGe2O6, here the Cu2+ cations occupies the M2 site; this may have a considerable impact on physical properties. Here we report the synthesis based on the preparation of a precursor by a soft chemistry method and detailed structural analysis of Cu0.8Mg1.2Si2O6, which can bring valuable insight into the role of the Jahn-Teller effects in metal site selectivity, structure distortion and chemical composition in pyroxene compounds.
reduction of Cu2+ to Cu1+, known to occur at ∼1020°C in air. A thermogravimetrical (TG and DSC) analysis was carried out using a Netzsch Thermal Analysis System to investigate the behaviour of the precursor with varying temperature. TG-DSC curves were recorded for ∼20.9 mg of precursor powder placed in an alumina crucible, by warming and cooling at a rate of 10°C min−1 between RT and 800°C. A mixed atmosphere (Ar 80% and O2 20%) was used. Morphology and chemical composition were investigated by field-emission scanning electron microscopy (FESEM, Zeiss Ultraplus) equipped with an energy-dispersive X-ray spectrometer (EDX, Bruker). The sample was gold-coated prior to SEM and EDX analysis. The zero field cooling (ZFC) and field cooling (FC) temperature dependence of magnetic susceptibility for Cu0.8Mg1.2Si2O6 was measured between 5 and 350 K on a Quantum Design, MPMS-XL SQUID magnetometer.
Powder X-ray diffraction
Experimental Sample preparation and characterization For a typical synthesis of 1 g of CuMgSi2O6 the stoechiometric quantities of Cu(C2H3O2)2.H2O, and tetraethoxysilane Mg(C2H3O2)2.4H2O, (TEOS: C8H20O4Si, 99.9%) were dissolved in 50 ml ethanol with vigorous stirring at 110°C for 3 h. The solution was dried at 60°C for several hours in order to remove solvents before further thermal treatment. The resulting precursor was calcined between 800°C and 1000°C (between 10 and 50 h, with intermediate regrinding) in air. This temperature range was chosen in order to avoid 326
All samples were characterized using powder X-ray diffraction (XRD) data collected with a Siemens D5000 diffractometer in transmission geometry, using a focusing Ge(111) monochromator for CuKα1 radiation and a linear PSD. For structure solution and refinement, a diffraction pattern was collected on the best sample obtained in terms of purity and crystallinity (sample n°6 in Table 1). Measurements were carried out at room temperature in the 10–90°2θ range with a step size of 0.032°. The Fox program (Favre-Nicolin and Cerny, 2002), was used to index the pattern, determine the most probable space group and provide a starting model for structure refinement, which was carried out by the Rietveld method using the Fullprof program (Rodríguez-Carvajal, 1993). Background was described by linear interpolation of selected points in the pattern. A Thomson-Cox-Hastings model (Thompson et al., 1987) of the reflection profile including anisotropic peak broadening was used. The size broadening effect was described using a uniaxial model with b as the unique axis, while a tensor description was applied for strain. Low-angle peak asymmetry was taken into account using the Bérar-Baldinozzi model (Bérar and Baldinozzi, 1993). In order to reduce the number of structural parameters, atoms of the same element were given equal isotropic displacement parameters. For the two metal sites, the composition was refined assuming
TABLE 1. Summary of synthesis conditions and resulting sample composition and pyroxene phase stoichiometry for CuMgSi2O6. Results and phases (wt.%) No.
1 2 3
Cu acetate, Mg acetate, TEOS Cu acetate, Mg acetate, TEOS Cu acetate, Mg acetate (>3 mol.%), TEOS Cu acetate, Mg acetate (>6 mol.%), TEOS Cu acetate, Mg acetate (>6 mol.%), TEOS Cu acetate, Mg acetate (>6 mol.%), TEOS Cu acetate, Mg acetate (>10 mol.%), TEOS Cu acetate, Mg acetate (>20 mol.%), TEOS
4 5 6 7 8
1000°C, 10 h 1000°C, 40 h 1000°C, 10 h
95.09(1.95) 93.91(1.47) 91.10(1.35)
1.48(0.19) 1.84(0.20) 1.12(0.19)
3.44(0.13) 4.25(0.15) 7.78(0.15)
0.79(2) 0.80(2) 0.79(2)
1.21(2) 1.20(2) 1.21(2)
1000°C, 10 h
1000°C, 50 h, regrinding 1000°C, 10 h
1000°C, 10 h